*Yu-Feng Jiang , Xue-Fei Hu , Uwamungu Yves and mechanisms of naphthalene adsorption by biochar...
Embed Size (px)
Transcript of *Yu-Feng Jiang , Xue-Fei Hu , Uwamungu Yves and mechanisms of naphthalene adsorption by biochar...
Effectiveness and mechanisms of naphthalene adsorption by biochar pyrolyzed from wheat straw
*Yu-Feng Jiang1) , Xue-Fei Hu2) , Uwamungu Yves3)
1), 2), 3) Department of Environmental Engineering, Lanzhou Jiaotong University, Lanzhou 730070, China
The objective of this study was to investigate the adsorption of naphthalene by biochar produced from pyrolytic wheat residue at varying temperature. The dynamic and thermodynamic adsorption experiments were conducted to investigate the adsorption characteristics of naphthalene by biochar. The result suggested that the surface feature and the chemical structure of biochar were modified at varying pyrolytic temperature. The kinetic data showed the adsorption of naphthalene onto biochar could be described by a pseudo-second-order kinetic model, and the boundary layer control and intraparticle diffusion are involved in the adsorption simultaneously. Besides, the adsorption thermodynamics fitted well with the Freundlich isothermal model. The saturated adsorption capacity was improved with the increase of systematic temperature, suggesting that adsorption was an endothermic process. Thermodynamic parameters analysis also showed the adsorption was mainly physical adsorption. The biochar produced by pyrolytic wheat residue showed a considerable potential for the naphthalene adsorption.
Keywords: Biochar, Pyrolysis, Adsorption, Thermodynamics, Naphthalene.
1. INTRODUCTION Biochar as a form of black carbon is a ubiquitous form of carbon comprising of polyaromatic to elemental or graphitic carbon, compared with organic carbon which forms covalent bonds with other elements (Chun et al. 2004; Lehmann and Joseph, 2009; Mohan et al., 2014). Biochar is quite similar to activated carbon with respect to mutual production via pyrolysis, with microporosity and high surface areas (Cao et al., 2011). Additionally, the biochar contains a non-carbonized fraction that may interact with organic pollutants. Specifically, the biochar also contains the carboxyl, hydroxyl, and phenolic surface functional groups that could effectively bind with pollutants (Mohan et al., 2014). Thus, biochar can be effective in sorption of organic pollutants such as dyes, aromatics, polychlorinated biphenyls, pesticides and petroleum hydrocarbons (Ahmad et al. 2012, 2013, 2014; Zhao et al. 2013; Zhang et al. 2013). Previous studies focus on 1) Professor 2) Graduate Student
adsorption of aqueous organic pollutants which mainly cover dyes, phenolics, pesticides, polynucelar aromatics and antibiotics (Ahmad et al. 2012, 2013, 2014; Mohan et al. 2014; Zhao et al. 2013; Zhang et al. 2013). But the surface properties and adsorptive characteristics may differ widely among biochar produced under varying conditions from different raw materials (Yang and Sheng, 2003; Ahmad et al. 2014; Mohan et al. 2014). Several mechanisms explaining the interactions between biochar and pollutants have been summarized (Ahmad et al. 2014). The major mechanisms controlling the fate of organic pollutants are the partitioning or adsorption because of biochars high surface area and microporosity, and electrostatic interaction between biochar and organic pollutants (Yang and Sheng, 2003; Uchimiya et al. 2010; Ahmad et al. 2012, 2013, 2014). Polar pollutants were adsorbed via the H-bonding between the pollutants and the O-containing moieties biochar (Sun et al. 2012; Uchimiya et al. 2011).
In Northwest China, because of petroleum industrial activities in the study areas, many petroleum pollutants are generated in the environment, deteriorating ecosystems. Therefore, understanding the adsorption behavior of petroleum pollutants is vital to predict their transport and fate in water. The primary objective of this study is to investigate the adsorption of naphthalene by biochar produced by pyrolyzing wheat residue at varying temperature. The kinetic and equilibrium data for the adsorption experiments were processed to understand the adsorption mechanism of naphthalene by biochar. 2. MATERIALS AND METHODS 2.1 Preparation of biochar samples Wheat residue was collected from farmland in Gansu province, China. The wheat residue was washed with distilled water four times, air-dried in a greenhouse for 2 days, and then oven-dried overnight at 80 . Some of treated wheat residue was weighed in a crucible, and covered with a fitting lid, then pyrolyzed under the oxygen-limited condition for 4 h at 200, 400, 600 C, respectively. During the heating process, the treated wheat residue was heated at 100 C for 1 h, and then increased temperatures to the corresponding temperature. The yield of each bio-product was defined as the ratio of the weight of the product to that of the original wheat residue. Under three pyrolytic temperatures (200, 400, and 600 C), the yields of biochar from the wheat residue were about 83%, 24%, and 21%, respectively. The biochar samples are hereafter referred to as BC-200, BC-400 and BC-600, respectively, where the suffix X00 (X = 2, 4, 6) to BC represents the pyrolytic temperature when the BC represent biochar. All biochar samples were sieved through 100 meshes.
The surface of char samples were scanned by JSM-5600LV low vacuum scanning electron microscope (SEM, Japan). For each analysis the voltage was set at 20 keV, while the working distance was 9 mm and the dead time for X-ray acquisition between 20% and 25%. Fourier transform infrared (FTIR) spectra were obtained using Bruker Vertex 70 spectrometer (Bruker Optics, Billerica, MA) fitted with a Pike Technologies MIRacle attenuated total reflectance (ATR) accessory (Madison, WI) with a diamond crystal plate. The spectra were obtained at 8 cm-1 resolution from 650 to 4500 cm-1 with 128 scans. Before FTIR analyses, all samples were adjusted to pH 3.0 and dried overnight at 70 C.
2.2 Adsorption experiments Adsorption kinetics and thermodynamics of naphthalene by biochar was
determined using a batch equilibrium method. Batch experiments of adsorption kinetics were conducted at 250.5 in an incubator shaker. A 0. 200 g of biochar samples was added to 100-mL plastic screw-capped bottles with 50 mL aqueous solution of naphthalene. The reaction mixture was incubated with stirring (140 rpm). The mixed samples were collected at reaction times of 0, 0.5, 1, 2, 6, 12, 20, 24, 36, 72 h, respectively, and then the solid and liquid were immediately separated at 4000 rpm by a centrifuge. The adsorption isotherm experiments were explained under constant agitation rate (140 rpm), initial pH (7.00.5), and three temperatures (25, 35, and 45 C), and it was conducted with an initial naphthalene concentration ranging from 0 to 48 mgL-1. The solid and liquid phases in all experiments were separated at 4000 rpm by a centrifuge after a given time. Finally the liquid phase was analyzed for naphthalene concentration by an UV spectrophotometer. All experiments were carried out in triplicate.
2.3 Adsorption kinetic model Kinetic adsorption is one major characteristic affecting the adsorption efficiency.
The kinetic data can be used to determine the presence or absence of intraparticle diffusion and whether it is the rate-controlling step. Three kinetic adsorption models including the pseudo-first-order, pseudo-second-order and intraparticle diffusion models were applied with the experimental data to predict the adsorption kinetics and mechanism.
The pseudo-first-order rate equation is expressed as follows (Ho and McKay 1998a; 1998b):
1 1 ( )t
kq q q t
where q1 and qt are the amounts of naphthalene adsorbed at equilibrium and at time t (mg g1) and k1 is the adsorption constant (min1).
The pseudo-second-order kinetic model (Ho and McKay 1998c) is expressed as:
22 2 2
1( )( )t
t tq q q k
where q2 is the maximum adsorption capacity (mg g1); qt is the amount of naphthalene adsorbed at equilibrium at time t (mg g1); k2 is the equilibrium rate constant (g mg1 min1).
The intraparticle diffusion equation (Weber Jr. and Morriss 1963) is written as follows:
t pq k t C (3)
where C is the intercept and kp is the rate constant (mg g1 min1/2). 2.4 Adsorption thermodynamic model
The equilibrium adsorption isotherms are one major type of data for understanding the adsorption mechanism (zcan et al. 2005). Three isotherm equations (Freundlichs, Langmuirs, and Dubinin- Radushkevich, D-R) were chosen in this study.
Langmuir adsorption model is based on the assumption that the maximum adsorption corresponds to a saturated monolayer of molecules on the adsorbent surface, with no lateral interaction between adsorbed molecules (Langmuir 1918). The Langmuir equation for homogenous surface is expressed as follows:
1 1 1
s L m e mc K q c q
where cs is the adsorption quantity of naphthalene by biochar (mgg-1); qm is the saturated adsorption quantity of naphthalene by biochar (mgg-1); ce is the equilibrium concentration of naphthalene in aqueous solution, mgL-1; KL is Langmuir thermodynamic equilibrium constant.
The Freundlich isotherm model is an empirical equation used to describe heterogeneous surfaces (Freundlich 1906):
1lg lg lgs F eq K cn (5)
where cs is the adsorption quantity of naphthalene by biochar (mgg-1); ce is the equilibrium concentration of naphthalene in aqueous solution (mgL-1); KF and n are constants related to biochar properties.
The equilibrium data were also processed by the D-R model to determine the nat